HAL Id: hal-01159400
Submitted on 3 Jun 2015
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Non-aqueous gel polymer electrolyte with phosphoric
acid ester and its application for quasi solid-state
Anna A. Łatoszyńska, Grażyna Zofia Żukowska, Iwona A. Rutkowska,
Pierre-Louis Taberna, Patrice Simon, Pawel J. Kulesza, Wladyslaw Wieczorek
To cite this version:
Anna A. Łatoszyńska, Grażyna Zofia Żukowska, Iwona A. Rutkowska, Pierre-Louis Taberna, Patrice
Simon, et al.. Non-aqueous gel polymer electrolyte with phosphoric acid ester and its application for
quasi solid-state supercapacitors. Journal of Power Sources, Elsevier, 2015, vol. 274, pp. 1147-1154.
Open Archive TOULOUSE Archive Ouverte (OATAO)
OATAO is an open access repository that collects the work of Toulouse researchers and
makes it freely available over the web where possible.
This is an author-deposited version published in :
Eprints ID : 13902
To link to this article
To cite this version
Ĕska, Anna A. and ĩukowska, GraĪyna
Zofia and Rutkowska, Iwona A. and Taberna, Pierre-Louis and Simon,
Patrice and Kulesza, Pawel J. and Wieczorek, Władysław
gel polymer electrolyte with phosphoric acid ester and its application
for quasi solid-state supercapacitors
. (2015) Journal of Power Sources,
vol. 274. pp. 1147-1154. ISSN 0378-7753
Any correspondance concerning this service should be sent to the repository
Non-aqueous gel polymer electrolyte with phosphoric acid ester and
its application for quasi solid-state supercapacitors
Anna A. Łatoszy
_zyna Zoﬁa _Zukowskaa
, Iwona A. Rutkowskab
, Patrice Simonc,d,**
, Pawel J. Kuleszab
, Władysław Wieczoreka
aFaculty of Chemistry, Warsaw University of Technology, Noakowskiego 3, 00-664 Warsaw, Poland bFaculty of Chemistry, University of Warsaw, Pasteura 1, 02-093 Warsaw, Poland
cUniversity Paul Sabatier, CIRIMAT, UMR-CNRS 5085, 31062 Toulouse Cedex 4, France dR eseau sur le Stockage Electrochimique de l'Energie (RS2E), FR CNRS n3459, France
h i g h l i g h t s
New proton-conducting gel polymer electrolyte has been proposed.
Electrochemical capacitor with new electrolyte has been assembled and tested in wide temperature operation range. The capacity value 120 F g!1has been reached at 22C and 83 F g!1at !40C.
Gel polymer electrolytes Phosphoric acid ester Electrochemical capacitor Wide temperature range
a b s t r a c t
A mechanically-stable non-aqueous proton-conducting gel polymer electrolyte that is based on meth-acrylate monomers, is considered here for application in solid-state type supercapacitors. An electro-chemical cell using activated carbon as active materials and the new gel polymer electrolyte has been characterized at room temperature using cyclic voltammetry, galvanostatic chargeedischarge cycle tests as well as impedance spectroscopy. The use of phosphoric acid ester (instead of phosphoric acid) as a proton donor has led to an increase of both the operation voltage window (up to 1.3 V) and the elec-trolyte ionic conductivity (on the level of an order of magnitude). The resulting double layer capacitance of the microporous activated carbon was found to be as high as 120 F g!1; even more important, the
supercapacitor utilizing non-aqueous proton-conducting gel polymer electrolyte is well-behaved in the wide temperature range (namely, from !40 to 80C).
There has been growing recent interest in electrochemical ca-pacitors (ECs) as high-power charge-storage devices that could possibly act as alternative or a complementary energy systems to conventional secondary batteries. In comparison to batteries, ECs are typically characterized by lower speciﬁc energy but much higher speciﬁc power, in addition to longer cycle life[1e5].
Among important issues, there is a need to improve the EC's energy density, which is related to capacitance according to Eq.(1).
E ¼1 = 2CV2 (1)
where C stands for capacitance (in F), V is the cell voltage (in V), and
E refers to energy (in J). A reasonable strategy for improving the
energy density is to use highly capacitive materials. Among different systems of potential utility for Electrochemical Double Layer Capacitors (EDLCs), such carbon materials as activated, tem-plated and carbide-derived carbons[6e9], carbon fabrics, ﬁbers, nanotubes[10,11], onions, nanohornsand graphene
have been considered. Highly effective pseudo-capacitive mate-rials, such as metal oxides (i.e. MnO2, RuO2, Nb2O5) or
conducting polymers (i.e. polyaniline (PANI), polypyrrole (PPy)
) that are characterized by fast electron transfers (between highly populated redox sites) responsible for their reversible charging/discharging processes, have also been proposed.
*Corresponding author. Faculty of Chemistry, Warsaw University of Technology, Noakowskiego 3, 00-664 Warsaw, Poland.
**Corresponding author. University Paul Sabatier, CIRIMAT, UMR-CNRS 5085, 31062 Toulouse Cedex 4, France.
E-mail addresses:firstname.lastname@example.org(A.A. Łatoszy nska),simon@chimie. ups-tlse.fr(P. Simon).
Another option for increasing the energy density is to enlarge the cell voltage that is often limited by the electrolyte decompo-sition at high potentials. Indeed, most of commercial super-capacitors utilize non-aqueous organic electrolytes and, consequently, they can reach cell voltage as high as 3 V and they can operate at temperatures ranging from !30C to 60C.
Despite of these advantages of liquid organic electrolytes, application of semi-solid e rather than liquid e systems would be particularly advantageous because many problems related to packing issues, corrosion, self-discharge or leakage currents
could be solved. But the key issue is to maintain high ionic con-ductivity as well as good contact at the electrolyteeelectrode interface. This requirement is of particular importance in a case of EDLCs where high surface area carbons are used as active materials. One of the solutions proposed to tackle these issues is the combi-nation of liquid and polymer electrolytes to form gel polymer electrolytes (GPEs)[20e23].
In comparison to solid organic or inorganic electrolytes, GPEs have several advantages that include processability and ﬂexibility of polymer matrices thus enabling the contact with the electrode surface. Hydrogels are gel electrolytes where an aqueous solution of KOH, H2SO4or H3PO4is swollen within a polymer matrix based on
poly(vinyl alcohol) (PVA) or polyacrylamide (PAAM) [24e26]. Thanks to their high ionic conductivity (~0.6 S cm!1), the proton-conducting hydrogel electrolytes have already been used for supercapacitor applications. Using gels based on PVA[27e30], Lian et al. demonstrated high-rate capability and cyclability thanks to high ionic conductivity of the PVA gel (0.02 S cm!1); however, the
use of non-porous carbons limited the cell capacitance and energy. Ste˛pniak et al. reported capacitance as high as 130 F g!1for
acti-vated carbons in PAAM based electrolytes together with H2SO4
aqueous solution. However, due to the presence of water, the operation voltage window (0.8 V) and indirectly the device energy density (3.5 Wh kg!1), as well as the operation temperature range
were deeply affected.
An important alternative arises from the possibility of replacing water as a solvent in proton-conducting gel-electrolytes with the combination of propylene carbonate (PC) and N,N-dimethylformamide (DMF). Consequently, both the stability windows (up to 1.5 V) and the temperature operation range (from !40 C to 80 C) can be improved [31,32]. Besides the
choice of solvent, both the polymer host and the proton donor are of high importance. The polymer matrix should be an inert element in GPE, so the monomers, which react with proton donor should be rejected. In the presence of strong acids, such as H2SO4
or H3PO4, the degradation of the CeO bond in polyethers or
polyalcohols is feasible; moreover, the stability window tends to decrease down to 1 V in the presence of H3Oþions. For instance,
Morita et al. prepared non-aqueous GPEs from poly(ethylene oxide)-modiﬁed polymethacrylate (PEO-PMA) matrix and anhy-drous H3PO4 . But the use of high concentration of
phos-phoric acid limited the electrolyte potential window down to 1 V. In this respect, it is reasonable to consider aryl phosphates as alternatives to orthophosphoric acid. Indeed, many phosphoric acid esters have strong acid properties: e.g. the pKa of
mono-phenyl phosphate value is even lower than that characteristic of phosphoric acid. In addition, such features as miscibility with polar solvents and chemical compatibility with polymers make phosphoric acid esters good candidates for the replacement of phosphoric acid in GPEs.
In the present work, we explore proton-conducting GPEs based on methacrylate copolymer matrix for application in Electro-chemical Double Layer Capacitors (EDLC). At ﬁrst, we report the preparation and physicochemical characterizations of the GPE in which phosphoric acid has been replaced by its ester (diphenyl
phosphate) as a proton donor. The ionic conductivity and mecha-nisms of proton transport have been studied using thermal stability analysis. Finally, the electrochemical characterization of a super-capacitor cell using activated carbon electrodes and the GPE elec-trolyte has been achieved in a large temperature range (from !40C to 80C).
Monomers: methyl methacrylate (MMA), 2-hydroxyethyl methacrylate (HEMA) (Sigma Aldrich); cross linking agent: tri-ethylene glycol dimethacrylate (TEGDM) (Sigma Aldrich); proton donor: diphenyl phosphate (DPhHPO4) (Sigma Aldrich, 99%)
Scheme 1; solvents: propylene carbonate (PC) (Sigma Aldrich, anhydrous) and N,N-dimethylformamide (DMF) (Sigma Aldrich, anhydrous) were used without further puriﬁcation. Radical poly-merization initiator: benzoyl peroxide (BP) (Sigma Aldrich) was recrystallized from chloroform and dried under vacuum. Carbon material: activated carbon YP-80F was from Kuraray Chemical Co., LTD (SSA ~ 2145 m2 g!1); and poly(vinylidene ﬂuo-rideehexaﬂuoropropylene) (PVdFeHFP) was used as a binder.
2.2. Preparation of the gel electrolyte
Gel polymer electrolyte (GPE) was prepared in a glove-box un-der Ar atmosphere by mixing PC with monomers (MMA and HEMA), the initiator (BP) and the cross-linking agent (TEGDM). After stirring for 1 h, the solution was cast as a thin ﬁlm (~200
mm) on a glass plate and placed in oven at 60e70C for gelation (12 h).
The next step was soaking the ﬁlm with a solution of DPhHPO4in
DMF and left for 1 week. Various electrolytes were prepared, con-taining 12.5 wt.% polymer matrix (HEMA:MMA ratio of 60:40 wt.%), various concentrations of DPhHPO4(from 5 to 40 wt.% in the ﬁnal
concentration of GPEs), and solvent mixture (PC:DMF ratio of 70:30 wt.%). Appropriate amounts of BP (1 wt.%) and TEGDM (5 wt.%).
2.3. Electrodes and cell preparation
The composite carbon electrodes were prepared by mixing the activated carbon with 5 wt.% PVdFeHFP binder in acetone. The activated carbon was a YP-80F from the Kuraray company. It is a microporous carbon, with a high speciﬁc surface area of 2145 ± 16 m2g!1. Ar gas sorption measurements have shown that
the carbon structure contains mainly micropores (pore diameter lower than 2 nm), accounting for 87% of the total pore volume and mesopores in the 2e7 nm diameter range. 50% of the micropores is lower than 1 nm. The slurry was casted onto Au disks (thickness, ~60
mm; surface area, ~1.29 cm2), placed in vacuum oven and dried at 120C. The carbon mass loading was 2.0 mg cm!2. Symmetric
cells were assembled using Swagelok®
, and GPE was placed be-tween two opposing electrodes. To improve the contact bebe-tween electrode and solid electrolyte, carbon electrodes were wetted with few drops of solvent mixture (in which DMF was on 30 wt.% level).
2.4. Experimental techniques
Ionic conductivity was determined using an impedance spec-troscopy method (EIS) in the temperature range from !30 to 90C.
The samples were sandwiched between two stainless steel block-ing electrodes and placed in the temperature-controlled thermo-stat. Electrochemical measurements were done using a VMP Multichannel Potentiostat (VMP, Biologic Science Instrument, France) over the frequency ranging from 10 to 500 kHz.
The infrared (IR) spectra were recorded with a computer-interfaced Perkin Elmer 2000 FT-IR system in the wave number range from 400 cm!1to 4000 cm!1. The electrolytes were
sand-wiched between two NaCl pellets.
Differential Scanning Calorimetry (DSC) studies were performed in the !150 to 150C temperature range using DSC Q200 V24.2
Build 107 system equipped with low-temperature measuring head and liquid helium cooling element. Samples were loaded into aluminum pans and stabilized by cooling from the room temper-ature down to !150C. Samples were then heated at 20C min!1
rate up to 150C; an empty pan was used as a reference.
Electrochemical measurements were achieved at various tem-peratures (ranging from from !40 to 80C) using a Votsch climatic
chamber (Germany). Before starting electrochemical measure-ments, the cells were kept for 4 h until the desired temperature was reached, which was found to ensure that the cell temperature was the same as that of the chamber. Electrochemical impedance spectroscopy measurements of capacitor cells were achieved be-tween 100 kHz and 1 mHz. Cycling voltammetry (CV) experiments were performed at the scan rates of 1, 5 and 10 mV s!1; and the
constant current charge/discharge tests (GCPL) were carried upon application of 0.075 A g!1.
The gravimetric capacitance Camof active material (in F g!1) was
calculated from the cell capacitance (C) using the equation:
where mam was the weight of the active material (carbon) per
The cell capacitance was calculated by measuring the slope of a charge Q, versus voltage V plot. Charge was calculated from the integration of the CV plots recorded during the discharge step. The cell capacitance was also calculated from the slope of the galva-nostatic discharge plots using the equation below:
C ¼ I
where C was the capacitance of the cell (in F), I was the discharge current (in A), and dV/dt was a slope of the discharge curve (in V s!1).
3. Results and discussion
3.1. Electrolyte characterization
Prepared methacrylate-based polymer gel electrolytes are transparent and freestanding membranes (Fig. 1); they show high ﬂexibility and good mechanical stability. The elastic properties depend on the solvent contentand the main role of polymer matrix is to assure good structural integrity . It is generally accepted that the ion conduction mechanism in gel electrolytes is similar to that of liquid systems. In other words, the solvent acts as the main conduction medium in the gel system. Although such important physical features of proton conducting gels, as high
dielectric constant, low viscosity and wide operation temperature range[36e38]should be appreciated, the possibility of the pro-tonation of solvent molecules by the proton dopant is the next important factor.
Two methacrylate monomers have been chosen in the present work: methyl methacrylate (MMA) and 2-hydroxyethyl methac-rylate (HEMA). HEMA is widely used for biocompatibility and hydrophilicity in separation techniques, chemical sensors and biomaterials[39e42]. Each monomer was used before as polymer matrix in proton conducting systems [31,43] and no reaction between PeOH group and polymer chain was noticed. However based on comparison of the proton conductivities in gel and liquid systems, the slight decrease was observed in a gel. The reason for lower conductivity in gel originates from entrapping of liquid phase in polymer matrix: this results in higher viscosity and decrease of the mobility of charge carries. It was shown that with decreasing the polymer content in gel, the conductivity increased, combined with the decrease in viscosity of samples
Fig. 2a illustrates the temperature dependence of conductivity recorded for the gel electrolyte utilizing P(HEMA-co-MMA), PCeDMF mixture (30 wt.% of DMF) doped with H3PO4 and
diphenyl phosphate (proton donor contents, 5 and 15 wt.%). Within the entire temperature range (from 20 to 90 C), the
conductivity values of GPE doped with phosphoric acid ester are higher than those obtained with H3PO4 (at the same mass
con-tent). The increase in conductivity can be explained by the in-crease in acidity of partial esters (in comparison to H3PO4). The
substitution of acidic protons by aryl groups decreases the electron density on oxygen thus resulting in weakening of HeO bonds and increasing the acid dissociation.Fig. 2b shows the dependence of ionic conductivity as a function of inverse temperature recorded for gel electrolytes doped with diphenyl phosphate. Above tem-peratures ca. !20 C, the conductivity increases with the
con-centration of proton (from 5 to 40 wt.%). Below !20 C, the
decrease in conductivity with increasing proton concentration is observed.
The change of the conductivity with 1/T follows an Arrhenius's law; the values of activation energy (Ea) have been calculated using
Eq.(4)and collected inTable 1:
where, Eais the activation energy (in J mol!1), s∞¼ lim
kBis the Boltzmann constant (1.38 & 10!23 m2kg s!2K!1). The
activation energy value is one of the parameters helping to deﬁne the mechanism of proton transport. The previous works of Wiec-zorek et al. have pointed on PC and DMF as the most appropriate solvents. DMF is a protophilic solvent by itself that contributes to proton conduction according to the Grotthus-type proton-ex-change conduction transport. This mechanism leads to lowering the activation energy for proton conduction and increasing the conductivity. PC molecules cannot be easily protonate and, there-fore, the proton transport takes place via vehicle-type mechanism in this protophobic solvent; consequently, the charge carriers are polyatomic molecules of proton donor in the latter mechanism. The lower proton conductivity in PC based systems can be assigned to lower charge mobility because of the solvent's higher viscosity (2.5 cP) in comparison to DMF (0.8 cP).
The Eadecrease may suggest Grotthus e type mechanism to be
operative in the system. _Zukowska et al. examined the diphenyl phosphate based GPE with PC as a solvent. Comparison of the
Eadata (27.5 kJ mol!1for the proton donor concentration at 5 wt.%
level)obtained in the PC based GPE with results obtained in the PCeDMF solvents mixture (~18 kJ mol!1) (Table 1) clearly
in-dicates the decrease in mixed solvents. The Eavalues are consistent
with the protonation of DMF molecule taking place in the presence of the mixture of protophilic and protophobic solvents (Scheme 2). The proton transport is achieved via a Grotthus type mechanism, as previously observed in GPE with phosphoric acid as a proton donor
The FT-IR spectra of crystalline ester were obtained to get a better insight into the conduction mechanism. Because polymer matrix is not involved in the conduction mechanism, the spectra were compared to those of liquid solutions at the different ester contents in the PC-DMF solvents only.
The protonation of DMF particle, observed in the phosphoric acid based GPE, takes place also in esters. The broadening of the
yC]Opeak of solvent and a shift of this band, as well as shifts in the
positions of 1407 and 1094 cm!1peaks, typically attributed to
gCeHvibrations, were observed in acid solutions in pure DMF
. The FT-IR spectra taken for different mono- and diesters in DMF also conﬁrmed protonation of DMF particle. However, in solvent mixtures, the content of DMF is rather too small and any signiﬁcant changes were observed even with the highest ester
Conductivities of polymer electrolytes containing DPhHPO4solutions together with calculated activation energy values (Ea) and the glass transition temperatures determinate
by DSC (Tg). Samples contains 12.5 wt.% of polymer matrix and PCeDMF (30 wt.% of DMF in solvent mixture).
Polymer matrix Solvent Diphenyl phosphate
concentration (wt.%) s(S cm!1) at 20C Ea(kJ mol!1) Tg(C) P (MMA-co-HEMA) (60 wt.% of HEMA) PCeDMF (30 wt.% of DMF) 5 2.7 & 10!4 16.4 !109 15 3.1 & 10!4 19.1 !93 30 4.2 & 10!4 18.6 !91 40 5.7 & 10!4 18.0 !83
Scheme 2. The mechanism of proton transport in DMF.
Fig. 2. Ionic conductivity electrolytes as a function of inverse temperature for the P(HEMA-co-MMA) based gel electrolytes containing different concentration of proton donor, where a) a comparison of H3PO4and DPhHPO4and b) different concentration of
DPhHPO4. Samples contains 12.5 wt.% of polymer (where 60 wt.% is HEMA and 40 wt.%
concentration. Therefore, to conﬁrm proton conducting mecha-nism, the spectra regions characteristic for P]O, PeOeC and PeOeH should be analyzed.
Fig. 3a illustrates the region between 1300 and 800 cm!1, cor-responding to vibrations characteristics of organic phosphates. In the spectra of diphenyl phosphate, the bands with the strong in-tensity can be distinguish and assigned to P]O, PeOeH and PeOeC stretching vibrations. The
yP]Oband appears at 1273 cm!1
in the solid compound; on the other hand, this band is largely masked by a stronger band of PC in a case of the solutions spectra. The appearance of a strong solvent band should be noted here. When compared to the pure component, a shift of
frequencies with increase of ester concentration (from 1200 to 1197 cm!1) can be observed (Fig. 3b). This change in the peak
po-sition is indicative of the loss of hydrogen bonds between the ester molecules, and it indirectly implies protonation of the solvent. In the ester solution (40 wt.%), the peaks corresponding to
yPOeC stretching can be observed and their positions are almost
unaffected. A band, that shall be attributed to PeOeC stretching vibrations of diphenyl phosphate, appears at 963 (in solid) and 938 cm-1(in solution containing the ester at 40 wt.%). The band position is not affected by the concentration of ester.
To comment on the operational temperature range and the electrolyte's thermal stability, Differential Scanning Calorimetry (DSC) measurements were done.Table 1 presents the DSC data obtained for polymer gel electrolytes containing the proton donor at different concentrations. The only phase transition occurring in the !150 to 150C temperature range is the glass
temperature transition, as demonstrated inFig. 4for the 15 wt.% DPhHPO4. The thermal properties of GPE are mostly affected by
the presence and concentrations of the solvent and the proton donor. In the present work, however, the solvent content was constant, so that the change in thermal properties reﬂected the concentration of the proton donor. The increase of the diphenyl phosphate concentration resulted in stiffening of the system (that presumably reﬂected interactions with solvent and polymer matrix), and thus leading to changes in Tg values. The lowest
value of Tgwere obtained for the sample containing 5% of ester,
and the increase of the proton donor content resulted in an in-crease in Tg.
3.2. Electrochemical double layer capacitor characterization
The proposed and synthesized GPE electrolytes (as described in Experimental section) were further used to assemble EDLC cells, namely by sandwiching the casted electrolytes between two acti-vated carbon electrodes. The semi-solid proton-conducting gel acted as mechanically stable separator. The system with a content
Fig. 4. DSC plot for P(HEMA-co-MMA) based electrolyte (where 12.5 wt.% is polymer matrix) with 15 wt.% of diphenyl phosphate content and PCeDMF solvent mixture. Fig. 3. A comparison of FTIR spectra of crystalline ester (dotted line) with
DPhHPO4-PC-DMF solutions containing different ester concentration a) region characteristic for ester vibrations b) the inﬂuence of a solvent on the position of diphenyl phosphate characteristic bands.
of 15 wt.% of diphenyl phosphate was selected because of its reasonable conductivity at low temperatures, 0.073 mS cm!1 at !20C (that was obviously higher than that found for the
sys-tems with higher ester content).
The YP-80F carbon used here has a theoretical speciﬁc surface area of 2145 ± 16 m2g!1. The carbon structures contain mainly
micropores (pore diameter lower than 2 nm) and mesopores in the 2e7 nm diameter range.
Fig. 5a illustrates the cyclic voltammetric response of the YP-80F carbon electrodes coexisting with the diphenyl phosphate-based GPE recorded in a supercapacitor (at 1 mV s!1) at room
Fig. 5. Room temperature electrochemical characterization of symmetrical super-capacitor with polymer gel electrolyte: a 3-electrode CV collected at 1 mV s!1(a) and
corresponding Nyquist plot (b).
Fig. 6. CV of symmetrical supercapacitor with polymer gel electrolyte carried out with different scan rate.
Capacitance of commercial porous carbon with proton con-ducting GPE at room temperature.
Scan rate (mV s!1) C
Fig. 7. Galvanostatic chargeedischarge curve for symmetrical supercapacitor cell with polymer gel electrolyte collected at room temperature: (a) capacitor cell, (b) positive electrode and (c) negative electrode.
temperature in the three-electrode mode. The minimum potential is found to be !0.7 V vs Ag pseudo-reference electrode, and the maximum one is 0.6 V (vs Agþ/Ag) thus leading to a maximum cell voltage of 1.3 V. The cathodic potential range is deﬁned by the reduction of protons, while the oxidation of the solvent limits the anodic potential range, as already reported by Reiter et al.. The carbon capacitance reaches 120 F g!1in our gel electrolyte, which is
probably one of the highest capacitances reported ever for the electrochemical capacitors utilizing microporous carbons in con-tact with gel electrolytes[20,23,45e47].
Fig. 5b shows the Nyquist plot of the cell (GPE electrolyte in contact with YP-80F carbon electrodes), obtained from the impedance data (performed at 22 ± 1C). The vertical increase of
the imaginary part of the impedance conﬁrms the capacitive nature of the electrochemical storage. The series resistance measured at high frequencies reaches the value of 95
Ucm2, which is higher than those reported by Schroeder et al. using ionic liquid-based
GPE, ILGPE. This observation reﬂected presumably the large thickness (200
mm) of our electrolyte and, obviously, the somewhat lower conductivity of our quasi-solid protonically-conducting GPE (0.3 mS cm!1) versus the (more solid) ILGPE (1.8 mS cm!1) at room temperature. It is noteworthy that decreasing the GPE thickness down to 100
mm would lead to improvement of the equivalent series resistance (ESR) value.
Fig. 6shows the cyclic voltammetries (CV) recorded at various scan rates (at 22 ± 1C) using a supercapacitor cell with YP-80F
carbons and our diphenyl phosphate based GPE. The CV plots have typical (rectangular shaped) capacitive signature. As expected, the gravimetric capacitance Camhas somewhat decreased with the
increasing scan rate, namely from 120 F g!1at 1 mV s!1to 90 F g!1 at 10 mV s!1(see alsoTable 2), this observation reﬂects lower ionic conductivity of GPE electrolytes in comparison to liquid ones.
Fig. 7shows the galvanostatic chargeedischarge plots for the cell (GPE electrolyte in contact with YP-80F carbon electrodes) recorded at 75 mA g!1in a three-electrode cell conﬁguration in the
potential range from 0 to 1.3 V. All chargingedischarging proﬁles (i.e. characteristic of the cell as well as of each electrode considered separately) show linear-like dependencies of the potential versus time. This observation is in agreement with the capacitive charge-storage mechanism and the capacitance obtained from cycling voltammetry (seeTable 3).
3.3. Electrochemical double layer capacitor performance at distinct temperatures
An important issue is the cell performance at different tempera-tures, particularly those extreme one.Fig. 8a shows the CVs recorded
Equivalent series resistance (ESR), speciﬁc capacitance value per gram of average mass (Cam) for the symmetrical supercapacitor obtained at different temperature.
Temperature (C) Cut-off potential (DE in V) ESR (Ucm2) Cam(F g!1) at 1 mV s!1 Cam(F g!1) at 74 mA g!1 !40 0e1.3 947 83 88 !20 0e1.3 350 101 104 RT 0e1.3 95 123 123 40 0e1.2 79 150 153 60 0e1.1 28 141 144 80 0e1.0 25 133 133
Fig. 8. Electrochemical characterization of symmetrical supercapacitor with polymer gel electrolyte: CVs collected at 1 mV s!1(a), corresponding EIS Nyquist plots (b) at T < 0C
at 1 mV s!1at various temperatures, namely !20 and !40C. The
electrochemical signatures are consistent with the typical capacitive behavior with a rectangular shape. The decrease in capacitance at !40C (80 F g!1versus 120 F g!1obtained at 22C) originates
from the reduced ion mobility at such low temperature. Neverthe-less, 70% of the initial room temperature capacitance is still retained at !40C which is remarkable feature of the proton-conducting GPE
electrolyte. The fact, that the Nyquist plot (Fig. 8b) shows a sizeable increase in the series resistance (950
Ucm2) at high frequencies at !40C relative to the analogous value at !20C (350
supports our view about the decrease of ionic conductivity. The results ofFig. 8c refer to the capacitance versus cell voltages, analogous dependencies as above, except that the experiments have been performed at higher temperatures, namely at 40, 60, and 80C. Obviously, the rectangular-type shapes of curves inFig. 8c are
consistent with capacitive signatures. The observed increase in capacitance following the increase of temperature reﬂects obvi-ously the temperature dependent increases in the ionic conduc-tivity or, in other words, results from the improved ionic mobilities at higher temperatures (see Fig. 2b). The smaller Cam value
observed at 80C most likely results from the partial DMF
evapo-ration (the solvent's boiling point is 153C). It is noteworthy
that, at 80C, the maximum system's voltage is effectively reduced
down to 1 V presumably due to increase of the solvent oxidation and reaction rates.Fig. 8d illustrates the Nyquist plots recorded at temperatures ranging from the room temperature (22C) up to
80C. The decrease in the series resistance from the initial value
measured at ambient conditions (95
Ucm2) down to a low value of 25
Ucm2 at 80C shall be noted and attributed to the system's
higher ionic conductivity at 80C (1.1 mS cm!1as shown inFig. 2a).
The proton-conducting Gel Polymer Electrolyte has been pro-posed, in which as a new proton source, diphenyl phosphate has been used. The application of phosphoric acid ester instead of acid allowed to increase operation voltage window up to 1.3 V (versus 1 V for H3PO4) and reach conductivity (at 20C 3.1 & 10!4S cm!1)
an order of magnitude higher than for acid. The mechanical prop-erties of GPE permitted to replace separator in capacitor cell.
The electrochemical characterization of EDLC with activated microporous carbon has been carried out with a new proton-conducting electrolyte. For the GPE electrolyte, the capacitance of about 120 F g!1 (at 22C), with the maximum voltage window
1.3 V, has been reached. Additionally, the application of organic solvents (PC, DMF) allowed to test capacitor cell in the extreme temperature range (between !40C and 80C). In the
measure-ments at !40C, the capacitance reached 80 F g!1, which
consti-tutes 70% of the value obtained at 22 C (120 F g!1). In higher
temperature measurements, at 80C, the obtained capacitance is
about 133 F g!1with the operation voltage window 1 V. The
tem-perature operation range is signiﬁcant wide, compared with elec-trolytes applied in EDLC ﬁeld before.
The study was supported within the frame of the MPD/2010/4 Project belonging to the MPD Programme of Foundation for Polish Science (co-ﬁnanced by the European Union, Regional Develop-ment Fund) as well as by the Ministry of Science and Higher Edu-cation e National Science Centre, Poland under the Project No. NN507322040.
P.S. acknowledges the funding from the European Research Council (ERC, Advanced Grant, ERC-2011-AdG, Project 291543 e IONACES), as well as the funding from the Chair of Excellence of the
Airbus Group Foundation “Embedded multi-functional materials” (2012e2017).
B.E. Conway, Electrochemical Supercapacitors e Scientiﬁc Fundamentals and Technological Applications, Kluwer Academic/Plenum Publisher, New York, 1999.
R. Kotz, M. Carlen, Electrochim. Acta 45 (2000) 2483e2498. A. Burke, J. Power Sour. 91 (2000) 37e50.
P. Simon, Y. Gogotsi, Nat. Mater. 7 (2008) 845e854.
E. Frackowiak, Q. Abbas, F. Beguin, J. Energy Chem. 22 (2013) 226e240.  J.C.T. Kyotani, Y. Gogotsi. Carbon Materials for Electrochemical Energy Storage
Systems, CRC/Taylor and Francis.
M. Arulepp, J. Leis, M. Latt, F. Miller, K. Rumma, E. Lust, A.F. Burke, J. Power Sour. 162 (2006) 1460e1466.
J. Leis, M. Arulepp, A. Kuura, M. Laett, E. Lust, Carbon 44 (2006) 2122e2129. J. Chmiola, C. Portet, P.L. Taberna, P. Simon, G. Yushin, Y. Gogotsi, Abstracts of
Papers of the American Chemical Society, vol. 231, 2006.
 D.N. Futaba, K. Hata, T. Yamada, T. Hiraoka, Y. Hayamizu, Y. Kakudate, O. Tanaike, H. Hatori, M. Yumura, S. Iijima, Nat. Mater. 5 (2006) 987e994.  M. Noked, S. Okashy, T. Zimrin, D. Aurbach, Carbon 58 (2013) 134e138.  C. Portet, J. Chmiola, Y. Gogotsi, S. Park, K. Lian, Electrochim. Acta 53 (2008)
 C.-M. Yang, Y.-J. Kim, M. Endo, H. Kanoh, M. Yudasaka, S. Iijima, K. Kaneko, J. Am. Chem. Soc. 129 (2007) 20e21.
 W.-Y. Tsai, R. Lin, S. Murali, L.L. Zhang, J.K. McDonough, R.S. Ruoff, P.-L. Taberna, Y. Gogotsi, P. Simon, Nano Energy 2 (2013) 403e411.
 M.-W. Xu, D.-D. Zhao, S.-J. Bao, H.-L. Li, J. Solid State Electrochem. 11 (2007) 1101e1107.
 M. Skunik-Nuckowska, K. Grzejszczyk, P.J. Kulesza, L. Yang, N. Vlachopoulos, L. Haggman, E. Johansson, A. Hagfeldt, J. Power Sour. 234 (2013) 91e99.  V. Augustyn, J. Come, M.A. Lowe, J.W. Kim, P.-L. Taberna, S.H. Tolbert,
H.D. Abruna, P. Simon, B. Dunn, Nat. Mater. 12 (2013) 518e522.
 V. Khomenko, E. Frackowiak, F. Beguin, Electrochim. Acta 50 (2005) 2499e2506.
 R.J. Latham, S.E. Rowlands, W.S. Schlindwein, Solid State Ion. 147 (2002) 243e248.
 W. Lu, K. Henry, C. Turchi, J. Pellegrino, J. Electrochem. Soc. 155 (2008) A361eA367.
 G.P. Pandey, S.A. Hashmi, Electrochim. Acta 105 (2013) 333e341.  P. Staiti, F. Lufrano, Electrochim. Acta 53 (2007) 710e719.
 M. Schroeder, P. Isken, M. Winter, S. Passerini, A. Lex-Balducci, A. Balducci, J. Electrochem. Soc. 160 (2013) A1753eA1758.
 I. Stepniak, A. Ciszewski, Electrochim. Acta 56 (2011) 2477e2482.  H. Yu, J. Wu, L. Fan, Y. Lin, K. Xu, Z. Tang, C. Cheng, S. Tang, J. Lin, M. Huang,
Z. Lan, J. Power Sour. 198 (2012) 402e407.
 Z. Sun, A. Yuan, Chin. J. Chem. Eng. 17 (2009) 150e155.  H. Gao, K. Lian, J. Electrochem. Soc. 158 (2011) A1371eA1378.  H. Gao, K. Lian, J. Power Sour. 196 (2011) 8855e8857.  H. Gao, K. Lian, J. Mater. Chem. 22 (2012) 21272e21278.  H. Gao, H. Wu, K. Lian, Electrochem. Commun. 17 (2012) 48e51.
 D. Raducha, W. Wieczorek, Z. Florjanczyk, J.R. Stevens, J. Phys. Chem. 100 (1996) 20126e20133.
 J.R. Stevens, W. Wieczorek, D. Raducha, K.R. Jeffrey, Solid State Ion. 97 (1997) 347e358.
 M. Morita, J.L. Qiao, N. Yoshimoto, M. Ishikawa, Electrochim. Acta 50 (2004) 837e841.
 G. Zukowska, W. Wieczorek, M. Kedzierski, Z. Florjanczyk, Solid State Ion. 144 (2001) 163e173.
 R. Lin, P.-L. Taberna, S. Fantini, V. Presser, C.R. Perez, F. Malbosc, N.L. Rupesinghe, K.B.K. Teo, Y. Gogotsi, P. Simon, J. Phys. Chem. Lett. 2 (2011) 2396e2401.
 W. Wieczorek, G. Zukowska, R. Borkowska, S.H. Chung, S. Greenbaum, Elec-trochim. Acta 46 (2001) 1427e1438.
 J.C. Lassegues, Proton Conductors: Solid, Membranes and Gel e Materials and Devices, Cambridge University Press, Cambridge, 1992.
 K.D. Kreuer, Chem. Mater. 8 (1996) 610e641.
 C. Yu, M.H. Davey, F. Svec, J.M.J. Frechet, Anal. Chem. 73 (2001) 5088e5096.  Y. Sakai, M. Matuguchi, Y. Sadaoka, K. Hirayama, J. Electrochem. Soc. 140
 M. Pradny, P. Lesny, J. Fiala, J. Vacik, M. Slouf, J. Michalek, E. Sykova, Collect. Czechoslov. Chem. Commun. 68 (2003) 812e822.
 D. Cohn, A.S. Hoffman, B.D. Ratner, J. Appl. Polym. Sci. 29 (1984) 2645e2663.  J. Reiter, J. Velicka, M. Mika, Electrochim. Acta 53 (2008) 7769e7774.  L.I. Katzin, G.W. Mason, D.F. Peppard, Spectrochim. Acta Part A Mol. Biomol.
Spectrosc. 34 (1978) 57e61.
 R.L. Lavall, R.S. Borges, H.D.R. Calado, C. Welter, J.P.C. Trigueiro, J. Rieumont, B.R.A. Neves, G.G. Silva, J. Power Sour. 177 (2008) 652e659.
 C.-P. Tien, W.-J. Liang, P.-L. Kuo, H.-S. Teng, Electrochim. Acta 53 (2008) 4505e4511.
 M. Yamagata, K. Soeda, S. Ikebe, S. Yamazaki, M. Ishikawa, Electrochim. Acta 100 (2013) 275e280.